## 2 Materials and Methods
### Materials
\begin{table}
\begin{tabular}{c c c c c c c c c} \hline \hline \multirow{2}{*}{**Assembly**} & **Layer** & \multirow{2}{*}{**Textile**} & \multirow{2}{*}{**Weave**} & \multirow{2}{*}{**Raw Material**} & \multicolumn{2}{c}{**Thickness**} & \multicolumn{2}{c}{**Surface**} & \multirow{2}{*}{**Porosity**} & \multirow{2}{*}{**Yarn**} \\  & **Type** & & & & & **[mm]** & & **[g\(\cdot\)m\({}^{-2}\)]** & & **[\%]** \\ \hline \multirow{8}{*}{_A_} & Outer & Woven & plain & \multirow{2}{*}{ramid} & \multirow{2}{*}{0.495} & \multirow{2}{*}{199} & \multirow{2}{*}{67} & \multirow{2}{*}{31} \\  & shell & fabric 1 & & & & & & & \\ \cline{1-1}  & Moisture & Membrane 1 & - & polyurethane & 0.066 & & & 0.05 & - \\  & barrier & Nonwoven & - & & & 0.830 & & & 90 & - \\  & & fabric 1 & & & & & & & \\ \cline{1-1}  & Thermal & \multirow{2}{*}{PCM insert} & \multirow{2}{*}{-} & polyurethane & \multirow{2}{*}{4.467} & \multirow{2}{*}{6.269} & \multirow{2}{*}{1548} & \multirow{2}{*}{67} & \multirow{2}{*}{75} \\  & barrier & PCM insert & - & & & & & & \\  & & fabric 2 & & & & & & & \\ \hline \multirow{8}{*}{_B_} & Outer & Woven & \multirow{2}{*}{plain} & \multirow{2}{*}{ramid} & \multirow{2}{*}{0.411} & \multirow{2}{*}{192} & \multirow{2}{*}{47} & \multirow{2}{*}{12} \\  & shell & fabric 1 & & & & & & & \\ \cline{1-1}  & Moisture & Membrane 1 & - & polyurethane & 0.066 & & & 0.05 & - \\  & barrier & Nonwoven & - & & & 0.830 & & 155 & 90 & - \\  & Thermal & \multirow{2}{*}{PP insert} & \multirow{2}{*}{-} & polypropylene & \multirow{2}{*}{4.438} & \multirow{2}{*}{1308} & \multirow{2}{*}{70} & \multirow{2}{*}{-} \\  & barrier & & & & & & & & \\ \cline{1-1}  & & \multirow{2}{*}{Lining} & Woven & \multirow{2}{*}{plain} & \multirow{2}{*}{ramid} & \multirow{2}{*}{0.411} & \multirow{2}{*}{192} & \multirow{2}{*}{47} & \multirow{2}{*}{12} \\  & shell & fabric 1 & & & & & & & \\ \cline{1-1}  & Membrane 2 & - & polyurethane & 0.032 & & & & 0.07 & - \\ \cline{1-1}  & barrier & Nonwoven & - & & & & & & & \\ \cline{1-1}  & Thermal & \multirow{2}{*}{PCM insert} & \multirow{2}{*}{none} & \multirow{2}{*}{pouurethane} & \multirow{2}{*}{4.467} & \multirow{2}{*}{1548} & \multirow{2}{*}{67} & \multirow{2}{*}{-} \\  & barrier & PCM insert & - & & & & & & \\ \cline{1-1}  & & fabric 2 & & & & & & & \\ \cline{1-1}  & & \multirow{2}{*}{Lining} & Woven & \multirow{2}{*}{plain} & \multirow{2}{*}{ramid} & \multirow{2}{*}{0.411} & \multirow{2}{*}{192} & \multirow{2}{*}{47} & \multirow{2}{*}{12} \\  & shell & fabric 1 & & & & & & & \\ \cline{1-1}  & & Membrane 2 & - & polyurethane & 0.032 & & & 0.07 & - \\ \cline{1-1}  & & Nonwoven & - & & & & & & \\ \cline{1-1}  & barrier & \multirow{2}{*}{PP insert} & \multirow{2}{*}{-} & \multirow{2}{*}{polypropylene} & \multirow{2}{*}{4.438} & \multirow{2}{*}{1308} & \multirow{2}{*}{70} & \multirow{2}{*}{-} \\ \cline{1-1}  & & barrier & & & & & & & \\ \cline{1-1}  & & \multirow{2}{*}{Woven} & \multirow{2}{*}{plain} & \multirow{2}{*}{ramid} & \multirow{2}{*}{0.411} & \multirow{2}{*}{192} & \multirow{2}{*}{47} & \multirow{2}{*}{12} \\ \cline{1-1}  & & \multirow{2}{*}{fabric 2} & & & & & & & \\ \cline{1-1}  & & \multirow{2}{*}{fabric 2} & & & & & & & \\ \hline \hline \end{tabular}
\end{table} 
Table 2: Characteristics of four tested assemblies. tested assemblies was intended to clearly distinguish the pair of assemblies \(A\) and \(C\) from the pair of assemblies \(B\) and \(D\) in terms of spatial structure. Nonwoven fabric 2 forming the moisture barrier in assemblies \(C\) and \(D\) was 52% thinner and 12% less porous than the nonwoven fabric 1, forming the moisture barrier in assemblies \(A\) and \(B\).